• Tidak ada hasil yang ditemukan

Directory UMM :Journals:Journal_of_mathematics:OTHER:

N/A
N/A
Protected

Academic year: 2017

Membagikan "Directory UMM :Journals:Journal_of_mathematics:OTHER:"

Copied!
12
0
0

Teks penuh

(1)

Geom., Cont. and Micros., I

RATE-INDEPENDENT PLASTICITY

Abstract. Work hardening in crystalline materials is related to the accumulation of statistically stored dislocations in low-energy structures. We present here a model which includes dislocation dynamics in the rate-independent setting for plasticity. Three basic physical features are taken into account: (i) the role of dislocation densities in hardening; (ii) the relations between the slip velocities and the mobility of gliding dislocations; (iii)the energetics of self and mutual interactions between dislocations. The model unifies a number of different approaches to the problem presented in literature. Reaction-diffusion equation with mobility depending on the slip velocities are obtained for the evolution of the dislocations responsible of hardening.

1. Introduction

Slip lines and slip bands on the surface of a plastically deformed crystal are due to complicated phenomena which occur inside the crystal. When plastic deformation occurs, dislocations are generated : some of them move towards the crystal surface forming slip lines, others may be stored to harden the material and form more or less regular patterns ([1]-[16]). As reported in Fleck et al. [1], “dislocations become stored for two reasons : they accumulate by trapping each other in a random way or they are required for compatible deformation of various parts of the crystal. The dislocation which trap each other randomly are referred to as statistically

stored dislocations...gradients of plastic shear result in the storage of geometrically necessary dislocations”.

Taking into account both statistically stored dislocation (SSD) and geometrically necessary dislocations (GND), our purpose in this paper is to construct a model which is able, at least in the simple case of single slip, to describe dislocations patterns. The basic idea here is to introduce dislocation densities as independent variables in the framework of Gurtin’s theory of gradient plasticity [17].

Total dislocation densities have been introduced frequently in the literature, both to describe hardening and the formation of patterns during plastic deformations ([18]-[26]).

In fact, materials scientists often describe hardening due to dislocation accumulation by means of the so-called Kocks’ model (see [22]): the resistance to slipζis assumed to depend on the total dislocation density̺through a relation of the form

ζ=ζ (̺),

∗This paper has been completed with the support of the Italian M.U.R.S.T. 1998-2000 research project “Modelli matematici per la scienza dei materiali”. We also wish to thank M.E. Gurtin, for his stimulating comments and suggestions.

(2)

and the accumulation of dislocations during plastic slip evolves according to an ordinary differ-ential equation which can be rewritten in the form

(1) d̺

dt = |ν|(ks

̺−kr̺),

whereνis the resolved (plastic) shear strain rate and kr, ksare positive constants. In the right

hand side of equation (1), the term ks√̺represents dislocation storage and the terms kr̺

repre-sents dynamic recovery. An important consequence of this approach is immediately recognizable by equation (1): the dislocation rate̺˙ depends on the strain rate. Roughly, this means that dis-locations are less mobile when the material hardens.

The above approach does not take into account dislocation density gradients and thus, while very efficient for small strain rates, it does not allow to study spatial variations of the density. One of the first approaches to non-local models, which should take into account both spatial and temporal variations of the dislocation density, is due to Holt [18], which obtains a Cahn-Hilliard equation for the total dislocation densities to describe patterning in a manner analogous to spinoidal decomposition in alloys. His model is based on a free energy density which takes into account dislocation interactions through higher gradients of the dislocation density, in con-junction with a gradient-flow derivation of a balance equation for such densities.

Other authors, for instance Aifantis (see for example [23]) and co-workers, model the com-plex phenomena due to dislocation interaction and annihilation by means of a reaction-diffusion system: in this approach two or more dislocation species are involved (e.g., mobile and immobile dislocations) and an evolution equation for each specie, say̺(X,t), is postulated

(2) d̺

dt =D1̺+g(̺)

where g(̺)is a source term describing creation and annihilation of dislocations (e.g., g(̺)= a̺−b̺2, with a and b phenomenological coefficients), D is a diffusive-like coefficient and1 is the laplacian. Models like (2) may be used to describe various phenomena related to pattern formation, but they do not include (plastic) strain rate effects of the type described by (1).

The main goal of our work is a unified model which includes all the basic features of the models described above, i.e., the dependence of (plastic) shear rate on dislocation density rate, the non-locality, and finally a term describing work and soft-hardening.

Using consistently the assumption of rate-independence (see Gurtin [17]), we obtain an equation for the total edge dislocation density of the form

(3) d̺

dt = |ν|

ǫ1̺ ∂ϕ ∂̺

whereǫmay be interpreted as a diffusive coefficient andϕ(̺)is a dislocation energy including work and soft-hardening behavior. Notice that equilibrium solutions satisfy

(4) ǫ1̺−∂ϕ

∂̺=0.

(3)

Ifτ andζ (̺)denote the resolved shear stress and the slip resistance respectively, then by regularization of the classical yield equationτ=(sgnν)ζ (̺), by lettingτ=(sgnν)|ν|1/nζ (̺)

for a large positive integer n, we obtain

(5) |ν| =

|τ| ζ (̺)

n .

By substitution ofν, as given by (5), into (3), we obtain the non linear parabolic differential equation

(6) d̺

dt =

|τ| ζ (̺)

n

ǫ1̺ ∂ϕ ∂̺

,

which can be solved if the resolved shear stressτ =τ (X,t)is known as a function of position and time.

2. Kinematics

Consider a body identified with its reference configurationBR, a regular region inR3, and let X∈BRdenote an arbitrary material point of the body. A motion of the body is a time-dependent one-to-one smooth mapping x = y(X,t). At each fixed time t , the deformation gradient is a tensor field defined by

(7) F=Grady

and consistent withdetF(X,t) >0 for any X inBR. A superposed dot denotes material time derivative so that, for instance,y is the velocity of the motion.˙

We assume that the classic elastic-plastic decomposition holds, i.e.,

(8) F=FeFp,

with Feand Fpthe elastic and plastic gradients, consistent with Je =detFe > 0 and Jp =

detFp > 0. The usual interpretation of these tensors is that Fe represents stretching and

rotation of the atomic lattice embedded in the body, while Fprepresents disarrangements due to

slip of atomic planes.

We restrict attention to plastic slip shear deformation, i.e., deformations such that the de-composition (8) holds, with Fearbitrary and with Fpof the form

(9) Fp=Ism, s·m=0,

with I the identity inR3, s and m constant unit vectors andα = α(X,t). In (9),α˙ may be interpreted as slip rate on the slip plane, defined by the glide direction s and the slip-plane normal m. This plane is understood to be the only one active among all the available slip systems.

2.1. The geometrically necessary dislocation tensor

(4)

DEFINITION1. Let S be a surface in the deformed configuration, whose boundaryS is a smooth closed curve. The Burgers vector ofS is defined as

b(∂S)= Z

S

Fe1dx

where dx is the line element of the circuitS. Stokes’ theorem implies that

b(∂S)= Z

S

curlFe1Tnda,

where n is the unit normal to the surface S andcurl and da are, respectively, the curl operator with respect to the point x and the area element in the deformed configuration.

SincecurlFe16=0 is necessary to have non null Burgers vectors, the tensorcurlFe1

seems to be a candidate to measure geometrically necessary dislocations. As such, however, it suffers some drawbacks: for example,curlFe1is not invariant under superposed compatible

elastic deformations; moreover, in view of applications to gradient theories of plasticity, it should be desirable to work in terms of a dislocation measure which can be expressed in terms of the plastic strain gradient also. In [27], Cermelli and Gurtin prove the existence of a dislocation tensor which satisfies both requirements above. We can rephrase their result as follows:

DEFINITION2. Let y be a deformation and F= ∇y its deformation gradient. If Feand Fp

are smooth fields satisfying (8), then the identity J1

pFpCurlFp=JeF −1

e curlFe1holds: we

define therefore the geometrically necessary dislocation tensor (GND tensor) as

(10) DG:= 1

Jp

FpCurlFp=JeFe−1curlFe1.

By (10), we have an alternative plastic and elastic representation of DG. As pointed out in

[27], in developing a constitutive theory “it would seem advantageous to use the representation of DGin terms of Fp, which characterizes defects, leaving Feto describe stretching and rotation

of the lattice”. See [27] for an exhaustive discussion of the geometrical dislocation tensor defined by (10).

For single slip plastic deformations (9), the GND tensor has the form

(11) DG=(∇α×m)⊗s=sgss+egts

where t=s×m and

(12) eg= ∇α·s, sg= −∇α·t.

The quantities egand sgcan be interpreted as densities associated to geometrically necessary

edge and screw dislocations, respectively, with Burgers vector parallel to s.

2.2. The total dislocation tensor

(5)

are present, and their line direction is contained in the slip plane m⊥, we introduce nonnegative functions

(13) e+=e+(X,t), e=e(X,t), s+=s+(X,t), s=s(X,t),

with the following interpretation : e+and eare the densities of dislocations with Burgers vector s and line direction t andt respectively (edge dislocations); s+and sare the densities of dislocations with Burgers vector s and line direction s ands respectively (screw dislocations).

Noting that all the information on a given system of dislocations may be summarized in one of the tensorial quantities (recall that e±, s± ≥0)

e+ts, −ets, s+ss, −sss,

we assume that the edge and screw densities above are related to the geometrically necessary dislocation tensor by a compatibility relation of the form

(14) DG=(e+−e−)ts+(s+−s−)ss from which it follows that

e+e= eg, s+−s−= sg.

DEFINITION3. Introducing the total edge and screw dislocation densities

e :=e++e, s :=s++s, we define the total dislocation tensor by

(15) DS:=e ts+s ss.

3. Dynamics

3.1. Standard forces and microforces

To describe the force systems associated to the motion of the body, plastic deformation and the evolution of the total dislocation densities, we introduce a tensor field S, vector fields bex t, ξ, κe

andκs, and scalar fields5, 5ex t, Me, Meex t, Msand Meex t, all functions of(X,t).

These fields correspond to three physically distinct sets of forces acting on the body. The first force system is standard, and is given by the usual Piola-Kirchhoff stress tensor S and the body force bex t.

The second force system has been introduced by Gurtin in his theory of gradient plasticity of single crystals (see [17]), to describe forces that perform work associated to plastic slip. This system consists in a vector microstressξ, a scalar internal microforce5, and a scalar external microforce5ex t.

The last set of forces is introduced to account for the dynamics of the total screw and edge dislocation densities. It consists of a vector forceκe, a scalar internal microforce Me, and a

scalar external microforce Meex tfor edge dislocations, and corresponding quantitiesκs, Ms and

Msex tfor screw dislocations.

A balance law is associated to each force system. We consider first the standard system (S,bex t), which is governed by the classical force balances, in local form given by

(6)

where we have omitted the inertial terms. To the second force system(ξ, 5, 5ex t), governing plastic slip, a corresponding microforce balance is associated (Gurtin, [17])

(17) Divξ+5+5ex t=0.

Following Gurtin, [17] we shall see later that this relation replaces the usual yield condition for the single slip system under consideration.

In our theory two more balances must be introduced, in order to obtain a complete integrable set of equations once an adequate constitutive theory is developed. These new balances are associated to the force systems(κe, 5e, 5ex te )and(κs, 5s, 5ex ts ), and are given in local form

by

Divκe+Me+Meex t =0,

Divκs+Ms+Msex t=0.

(18)

Each of the above force system is characterized by the way it expends power on the rate of change of the corresponding microstructural field : precisely, we assume that the working of the forces on an arbitrary portionPof the body is

W(P) = Z

∂P

(Sn· ˙y+ξ·nα˙ +κe·ne˙+κs·ns˙)da

+ Z

P

(bex t· ˙y+ ˙α5ex t+ ˙eMeex t+ ˙s Msex t)dv. (19)

Notice that the microstressξ and the corresponding external force, expend power on the slip velocityα˙, while the total dislocation forcesκeandκsexpand power on the rate of change of the

corresponding dislocation densities.

We take the second law in the form of a dissipation inequality, stating that the time-derivative of the free energy relative to an arbitrary subregionPof the body may not exceed the working of the external forces acting onP, i.e.,

(20) d

dt

Z

P

ψdv≤W(P)

whereψ is the free energy, density per unit volume in the reference configuration. Using the balance equations, this inequality becomes, in local form,

(21) ψ˙ ≤Te· ˙Fe+ξ· ∇ ˙α+κe· ∇ ˙es· ∇ ˙s+πα˙ −Mee˙−Mss˙

where

(22) Te=SFTp π=τ−5, τ=S·(Fesm).

Notice thatτis the resolved shear stress on the slip system under consideration.

3.2. Constitutive equations

Lettingσ =(Fe,e+,e,s+,s,∇e+,∇e,∇s+,∇s)andv=(α,˙ e˙,s˙)we consider

consti-tutive equations of the form

(7)

and

(24) π= ˆπ (σ, v), Me= ˆMe(σ, v), Ms = ˆMs(σ, v).

Requiring the consistency of the constitutive equations with the dissipation inequality for any process, we obtain by the classical Coleman-Noll procedure the result that the constitutive func-tions above cannot depend one+,e, s+ands, but only one ands, i.e., we can

rewrite the constitutive relations (23) in terms of the list

σ′=(Fe,e+,e−,s+,s−,∇e,∇s) or, equivalently,

σ′′=(Fe,eg,sg,e,s,∇e,∇s).

Furthermore, the constitutive relations in (23) must satisy the requirements

(25)

Te=

∂ψˆ ∂Fe

, ξ= ∂ψˆ

eg

s+ ∂ψˆ ∂sg

m×s, κe=

∂ψˆ

∂∇e, κs=

∂ψˆ ∂∇s,

while the internal microforces Meand Ms decompose as

(26) Me= −Medis

∂ψˆ

e, Ms = −M

dis s

∂ψˆ ∂s

where Medis, Msdisandπmust satisfy the residual dissipation inequality

(27) δ=πα˙+Medise˙+Msdiss˙≥0 for all processes(σ, v).

3.3. Rate independence

Notice that, under a time scale transformation defined by tt/θ,θ >0, the fieldsα,˙ e and˙ s˙ transform according toα˙ →θα,˙ e˙ →θe and˙ s˙ →θs. Following Gurtin, we assume that the˙ constitutive equations for Medis, Msdisandπare rate-independent, in the sense that they satisfy

Medis(σ, v)=Medis(σ, θ v), Msdis(σ, v)=Msdis(σ, θ v), π(σ, v)=π(σ, θ v), for any(σ, v)and for allθ >0.

4. A nonlinear model

For the applications presented in this paper, we choose a particular form of the free energy functionψ, namely

(28) ψ =ψe(Fe)+ϕ(eg,sg,e,s)+

1 2ǫ1|∇e|

2 +1

2ǫ2|∇s| 2

(8)

Moreover, we shall assume that the dissipative fields Medis, Msdisandπare given by ence, and yields a dissipation density1quadratic in the rates of change of the total dislocation densities. Moreover, as we shall see, whenα˙ =0, equations (29)1and (29)2are well-defined.

Following Gurtin [17], the functionζ may be interpreted as the slip resistance. In [17],ζ is introduced as internal variable, whose evolution is given by an ordinary differential equation, called the hardening equation, of the form

˙

ζ = f(λ,α),˙

whereλis a list possibly containing the fields Fe, Fp,∇Fp andζ. As shown in [17], when

restricted by rate independence, the hardening equation becomes

(30) ζ˙ =K(λ)| ˙α|.

Our approach to hardening is substantially different from that based on internal variables: we assume in fact thatζis given by a constitutive relation compatible with the dissipation inequality and the hypothesis of rate independence. Therefore it is not necessary to introduce the hardening equation a priori, since, as shown below, it is a consequence of the constitutive choices (29)1 and (29)2for Medisand Msdis.

To write explicitly the evolution equations for our model, we assume that no external forces are present, and choose a cartesian coordinate system(X,Y,Z)in the reference configuration such that

(1,0,0)=s×m (0,1,0)=s (0,0,1)=m. The balance equations are then

1) the balances of linear and angular momentum

(31) Div

Notice that the yield condition is modified by the presence of geometrically necessary dislocations (we have used (12) to express the geometrically necessary dislocation den-sities in terms of the derivatives of the plastic slipα), which can be thought as inducing isotropic hardening-softening.

3) a reaction-diffusion system for the total dislocation densities

(9)

Notice that the dislocation mobility is proportional to the modulus of the slip velocityα˙. Henceforth, two characteristic features of dislocation dynamics are immediately recog-nizable from (33):

(i) one can have equilibrium configurations for edge dislocations, i.e.,

ǫ11e

∂ϕ ∂e =0

such thate˙=0 and dislocations are ”locked” in low energy structures, but plastic flow does occur, and the slip velocity does not vanish:α˙ 6=0. A similar discussion applies to screw densities.

(ii) if the material behaves elastically, so thatα˙ =0, then dislocations cannot move. Besides, by derivations with respect the time of the constitutive relationζ (e,s)for the slip resistance, and using equations (33)1and (33)2, we obtain a hardening equation

(34) ζ˙ = which is a generalization of the classical equation (30).

5. One dimensional model

In this section we describe some simplifying assumptions which allow to reduce the reaction-diffusion system for the total dislocation densities, to a single one-dimensional equation for the total edge density.

ASSUMPTIONS

(i) We assume that the geometrically necessary dislocation densities vanish, i.e.,

eg=sg=0,

which implies that e+=e, s+=sand thus, by (12),αonly depends on(Z,t). (ii) Screw dislocations densities are assumed to vanish identically, and the total edge

disloca-tion density e is constant on each slip plane, so that e depends only on(Z,t). Thus e is the only non-vanishing dislocation density.

(iii) The resolved shear stressτis assumed to be constant with respect to(X,t). (iv) The constitutive relation for the slip resistance has the form

ζ (e)=ζ0+ce

whereζ0and c are positive constants. This relation is well known in the materials science literature (cf. Livingston [4], Van Drunen and Saimoto [5], Staker and Holt [6]). (v) We approximatesgnα˙ forα˙ 6=0 by

| ˙α|1nsgnα˙ with n large (viscoplastic regularization).

(vi) Assuming that the bodyBis an infinite layer between the planes Z =0 and Z= L, we

(10)

5.1. A particular energy dislocation function We further chooseϕ(e)in the form

(35) ϕ(e)= 1

4[e(eem)] 2,

with em >0 a constant. The functionϕ(e)is non-convex and non-negative with a local minimum

at e=0 and e=emand a local maximum at e=em/2.

5.2. The model

Assuming that the standard balance of momentum (31) is identically satisfied, the previous as-sumptions reduce the general model to the following two equations

(36) τ=(sgnα)˙ | ˙α|1/n(ζ0+c

e),

and

(37) e˙= 1

a| ˙α| ǫ1 ∂2e

Z2−e(eem/2)(eem)

! .

Using (36), equation (37) becomes

(38) e˙= 1

a

| ζ0+ce

n ǫ1

∂2e

Z2−e(eem/2)(eem) !

,

supplemented by the natural boundary conditions discussed above. Equation (38), which is the basic result of this work, is a non-linear partial differential equation which may be solved numerically: a complete discussion of the behavior of the solutions to (38) will be published elsewhere.

References

[1] FLECKN. A., MULLERG. M., ASHBYM. F.ANDHUTCHINSONJ. W., Strain gradient

plasticity: theory and experiment, Acta metall. mater. 42 (1994), 475–487.

[2] KUHLMANN-WILSDORFD., Modelling of plastic deformation via segmented voce curves,

linked to characteristic LEDS’s which are generated by LEDS transformation between workhardening stages, Phys. Stat. Sol. 149 (1995), 131–153.

[3] ASAROR. J., Micromechanics of crystals and polycrystals, Advances in Applied Mechan-ics 23, Academic Press, 1983.

[4] LIVINGSTONJ. D., The density and distribution of dislocation in deformed copper

crys-tals, Acta Met. 10 (1962), 229–239.

[5] VANDRUNENG.ANDSAIMOTOS., Deformation and recovery of [001] oriented copper

crystals, Acta Met. 19 (1971), 213–221.

[6] STAKERM. R. AND HOLTD. L., The dislocation cell size and dislocation density in

copper deformed at temperatures between 25 and 700C, Acta Met. 20 (1972), 567–579.

(11)

[8] FERNANDESJ. V.ANDSCHMITTJ. H., Dislocation microstructures in steel during deep

drawing, Phil. Magazine 48 A (1983), 841–870.

[9] KUHLMANN-WILSDORFD., Theory of plastic deformation:-properties of low energy

dis-location structures, Mater. Sci. Eng. 113 A (1989), 1–41.

[10] SWANNP. R., Dislocation arrangements in face-centred cubic metals and alloys, in: “The impact of the transmission electron microscopy on theories of the strength of crystals” Pro-ceeding of the First Berkeley International Materials Conference, University of California, July 5-8, Berkeley 1961.

[11] NEUMANNP., Low energy dislocation configurations: a possible key to the understanding

of fatigue, Mat. Sci. Eng. 81 (1986), 465-475.

[12] NABARROF. R. N., Theory of crystal dislocations, Clarendon Press, Oxford 1967.

[13] GLAZOV M., LLANES L. M. AND LAIRD C., Self-organized dislocation structures

(SODS) in fatigue metals, Phys. Stat. Sol. 149 b (1995), 297–321.

[14] N. HANSEN ANDHUGHESD. A., Analysis of large dislocation populations in deformed

metals, Phys. Stat. Sol. 149 b (1995), 155–171.

[15] ZAISERM.AND AIFANTISE. C., Material instabilities and deformation patterning in

plasticity, Recent Res. Devel. Metallurg. and Material Sci. 3 (1999), 79–103.

[16] ORTIZM.ANDREPETTOE. A., Nonconvex energy minimization and dislocation

struc-tures in ductile single crystals, J. Mech. Phys. Sol. 47 (1999), 397–462.

[17] GURTIN M., On the plasticity of single crystal: free energy, microforces, plastic-strain

gradients, J. Mech. and Phys. Sol. 48 (2000), 989–1036.

[18] HOLTL., Dislocation cell formation in metals, J. Appl. Phys. 41 8 (1970), 3197–3201.

[19] KRATOCHVILJ., Plastic properties and internal stability of deformed metals, Czech. J. Phys. 38 B (1988), 421–424.

[20] KRATOCHVILJ., Dislocation pattern formation in metals, Revue Phys. Appl. 23 (1988), 419–429.

[21] SUNS., ADAMSB. L., SHETC., SAIGALS.ANDKINGW., Mesoscale investigation of

the deformation field of an aluminium bicrystal, Scripta Materialia 39 (1998), 501–508.

[22] KOCKSU. F., Laws for work-hardening and low-temperature creep, J. Eng. Mate. Tech. (1976), 76–85.

[23] AIFANTISE. C., Pattern formation in plasticity, Int. J. Engng Sci. 33 (1995), 2161–2178.

[24] AIFANTISE. C., Gradient deformation models at Nano, Micro, and macro scales, J. Eng. Mater. Tech. 121 (1999), 189–202.

[25] AIFANTISE. C., The physics of plastic deformation, Inter. J. Plasticity 3 (1987), 211–247.

[26] SALAZAR J. M., FOURNET R. AND BANAI N., Dislocation patterns from

reaction-diffusion, Acta Metall. Mater. 43 (1995), 1127–1134.

[27] CERMELLIP.ANDGURTINM., On the characterisation of geometrically necessary

(12)

AMS Subject Classification: 74C05, 74C15. Luca BORTOLONI

Dipartimento di Matematica Universit`a di Bologna Piazza di Porta San Donato 5 40127 Bologna, ITALY

e-mail:bortolon@dm.unibo.it

Paolo CERMELLI

Dipartimento di Matematica Universit`a di Torino Via Carlo Alberto 10 10123 Torino, ITALY

Referensi

Dokumen terkait

[r]

f) Sertifikat keahlian (SKA) dan Ijazah tenaga ahli tetap yang dipersyaratkan, dan.. g) Surat pengangkatan tenaga ahli tetap bersangkutan oleh pimpinan perusahaan dan

[r]

In addition, Ball and King (2006) differentiate PPP and conventional procurement in three aspects. First, conven- tional procurement only includes infrastructure procure- ment in

Berdasarkan Perpres 54 Tahun 2010 beserta perubahannya dan aturan turunannya (Perpres Nomor 70 Tahun 2012 dan Perpres Nomor 04 Tahun 2015) serta Hasil Evaluasi

Dengan ini diumumkan Pemenang Pelelangan dan Pemenang Cadangan, adalah sebagai berikut

Dilihat dari perspektif keuangan secara keseluruhan kinerja CV Yamaha Sinar Utama Hidayatullah Samarinda pada tahun 2012 cukup baik, sedangkan pada tahun 2013

Menindaklanjuti proses evaluasi penawaran Pekerjaan Pembangunan Rumah Dinas Dokter RSUD Kaur pada Dinas Pekerjaan Umum Kabupaten Kaur, Pokja III ULP Kabupaten Kaur akan